Investigation of antibacterial properties silver nanoparticles prepared via green method
© Shameli et al.; licensee Chemistry Central Ltd. 2012
Received: 20 May 2012
Accepted: 10 July 2012
Published: 27 July 2012
This study aims to investigate the influence of different stirring times on antibacterial activity of silver nanoparticles in polyethylene glycol (PEG) suspension. The silver nanoparticles (Ag-NPs) were prepared by green synthesis method using green agents, polyethylene glycol (PEG) under moderate temperature at different stirring times. Silver nitrate (AgNO3) was taken as the metal precursor while PEG was used as the solid support and polymeric stabilizer. The antibacterial activity of different sizes of nanosilver was investigated against Gram–positive [Staphylococcus aureus] and Gram–negative bacteria [Salmonella typhimurium SL1344] by the disk diffusion method using Müeller–Hinton Agar.
Formation of Ag-NPs was determined by UV–vis spectroscopy where surface plasmon absorption maxima can be observed at 412–437 nm from the UV–vis spectrum. The synthesized nanoparticles were also characterized by X-ray diffraction (XRD). The peaks in the XRD pattern confirmed that the Ag-NPs possessed a face-centered cubic and peaks of contaminated crystalline phases were unable to be located. Transmission electron microscopy (TEM) revealed that Ag-NPs synthesized were in spherical shape. The optimum stirring time to synthesize smallest particle size was 6 hours with mean diameter of 11.23 nm. Zeta potential results indicate that the stability of the Ag-NPs is increases at the 6 h stirring time of reaction. The Fourier transform infrared (FT-IR) spectrum suggested the complexation present between PEG and Ag-NPs. The Ag-NPs in PEG were effective against all bacteria tested. Higher antibacterial activity was observed for Ag-NPs with smaller size. These suggest that Ag-NPs can be employed as an effective bacteria inhibitor and can be applied in medical field.
Ag-NPs were successfully synthesized in PEG suspension under moderate temperature at different stirring times. The study clearly showed that the Ag-NPs with different stirring times exhibit inhibition towards the tested gram-positive and gram-negative bacteria.
KeywordsSilver nanoparticles Green chemistry Polyethylene glycol Antibacterial activity Reaction time effect
Silver nanoparticles (Ag-NPs) have been known for its inhibitory and bactericidal effects in the past decades . Antibacterial activity of silver containing materials can be applied in medicine for reduction of infections on the burn treatment [2, 3], prevention of bacteria colonization on catheters [4, 5] and elimination of microorganisms on textile fabrics [6, 7] as well as disinfection in water treatment . Besides that, Ag-NPs were also being reported in the literature to exhibit a strong cytoprotective activity towards human immunodeficiency virus (HIV) infections . Polyethylene glycol (PEG) is frequently used in the polymer blends production to improve the biocompatibility of its film due to its wide range of molecular weights, excellent solubility in aqueous medium, low toxicity, chain flexibility and biocompatibility properties. Although PEG has non biodegradability properties, it is readily excreted from the body and forms non-toxic metabolites . Besides that, PEG was able to act both as reducing agent and stabilizer . In several research studies [12, 13], researchers proposed that longer polymer chain of PEG exhibits higher reducing activity and provides higher stability in forming Ag-NPs. These can effectively prevent agglomeration of Ag-NPs.
There are numerous techniques to perform antibacterial and antimicrobial susceptibility tests. The techniques include agar disk diffusion, broth dilution (macrodilution and microdilution), agar dilution and E test method (modification of the disk diffusion and the agar dilution method) . Agar disk diffusion is a traditional and routine method for antimicrobial susceptibility tests . It has advancement to be used in this project because of its reliability, low cost and simplicity [16, 17]. Mueller Hinton agar is chosen among the culture media because it gives satisfactory growth for most nonfastidious organisms like Staphylococcus aureus, Pseudomonas aeruginosa and Escherichia coli and it shows good bacteria culture reproducibility .
There are many synthetic routes that have been developed to synthesize Ag-NPs due to the applications found tremendously in wide range of fields. Among the synthetic routes includes chemical reduction [19, 20], thermal decomposition , electrochemical , sonochemical , photochemical , microwave , radiation assisted process [26, 27] and currently by green chemistry synthesis [28–31].
Chemical reduction method is widely used to synthesize Ag-NPs because of its readiness to generate Ag-NPs under gentle conditions and its ability to synthesize Ag-NPs on a large scale . However, these chemical synthesis methods employ toxic chemicals in the synthesis route which may have adverse effect in the medical applications and hazard to environment. Therefore, preparation of Ag-NPs by green synthesis approach has advantages over physical and chemical approaches as it is environmental friendly, cost effective and the most significant advantage is that conditions of high temperature, pressure, energy and toxic chemicals are not required in the synthesis protocol .
In this work, we reported “green” synthesis of Ag-NPs using sugar and PEG. This method was performed by reducing the silver nitrate (AgNO3) in different stirring times of reaction at moderate temperature with sugar and PEG used as green reducing agent and polymeric stabilizer. The antibacterial activity of silver/polyethylene glycol [Ag(PEG)] were tested with Mueller-Hinton agar disc diffusion method against Staphylococcus aureus (S. aureus), and Salmonella typhimurium SL1344 (S. typhimurium SL1344).
Results and discussion
After dispersion of silver ions in the PEG aqueous solution matrix (Equation 1), PEG reacted with the Ag to form a PEG complex [Ag(PEG]+, which reacted with sugar to form [Ag(PEG)] due to the reduction of silver ions through the oxidation of sugar to gluconic acid (Equation 2).
Thus, there is a normal case in this situation for the SPR absorption band for the particles, which agreed with the TEM results, whereby red–shifts were observed as size increased in the during the reaction after 1, 3, 6, 24 and 48 h respectively. This can be explained by the multilayer Mie theory model, which theorizes that the chemical interaction caused the lowered electron conductivity in the outermost atomic layer and consequently caused the red–shifts . As seen from the Figure 2C, it can be observed that 24 h had large absorbance compared to 48 h because the particle size of Ag-NPs after 48 h were larger than those at 24 h. Also, absorption spectra of larger metal colloidal dispersions can exhibit broad peaks or additional bands with the lower absorbance in the UV-visible range due to the excitation of plasma resonances or higher multipole plasmon excitation . This phenomenon could be due to the fact that, after reaching a certain particle size, the stabilizer was not able to withhold the nanoparticle’s size effectively, which resulted in its very large size.
Powder X–ray diffraction
Where K is the Scherrer constant with value from 0.9 to 1 (shape factor), where λ is the X-ray wavelength (1.5418 Å), β1/2 is the width of the XRD peak at half height and θ is the Bragg angle. From the Scherrer equation the average crystallite size of Ag-NPs for 6, 24 and 48 h times of reaction are found to be around 10–25 nm, which are also in line with the observation of the TEM results discussed later.
Zeta potential measurement
FT-IR chemical analysis
Thus, as shown hydroxyl group of PEG as capping agent can make a cover in the surface of Ag-NPs. This is possible because the surface of Ag-NPs is positively charged. Certainly, we suppose that colloidal stabilization for [Ag (PEG)] occur due to the presence of van der waals forces between the oxygen negatively charged groups present in the molecular structure of the PEG, and the positively charged that surround the surface of the inert Ag-NPs [45, 47]. Therefore, the FT-IR spectra showed the existence molecular interactions between the Ag-NPs with the chain of polymeric media . As shown in the Figure 6, schematic illustrated the interaction between the charged of Ag-NPs that capped with PEG [28, 48].
Average inhibition zone and standard deviation for PEG, [Ag (PEG)] + (A0) and [Ag (PEG)] suspension (A2–A5) at different stirring times (3, 6, 24 and 48 h), respectively
11.65 ± 0.56
12.78 ± 0.12
13.64 ± 0.29
9.71 ± 0.14
9.67 ± 0.33
9.44 ± 0.36
11.51 ± 0.43
10.64 ± 0.39
10.62 ± 0.36
In summary, we have described a simple and green method of colloidal Ag-NPs synthesis by using green reducing agents which requires no special physical conditions. Ag-NPs were successfully synthesized under moderate temperature (45°C) at different stirring times of reaction. The formation of Ag-NPs was confirmed in the UV-visible absorption spectra, which showed the SPR band characteristics of Ag-NPs in the range of 412–437 nm. The XRD results confirmed that the Ag-NPs possessed a face-centered cubic crystal structure (fcc). In addition, this also revealed that Ag-NPs were the main composition present in the nanocomposites without any contamination peaks. The TEM images showed that the Ag-NPs were in spherical shape and the average diameters of the particles were 10.60, 11.23, 12.95 and 25.31 nm for the stirring times of 3, 6, 24 and 48 h, respectively. FTIR spectrum suggested the complexation present between PEG and Ag-NPs to form metallopolymer [Ag (PEG)] and the stability of the Ag-NPs was confirmed with the zeta potential measurements. The antibacterial activities of [Ag (PEG)] at the different particle size of Ag-NPs were showed antibacterial activity against the Gram-positive and Gram-negative bacteria. These results show that the antibacterial activities of Ag-NPs in PEG can be modified with the size of Ag-NPs and it decreases with the increase in the particle size. Needless to say, further studies are required to investigate the biological effects of [Ag (PEG)] suspension on the types of bacteria for potential widening of this subject area.
All reagents in this effort were analytical grade and were used as received without further purification. AgNO3 (99.98%) was used as a silver precursor, and was provided by Merck, Germany. PEG (Mw 3,350) used as a stabilizer for the preparation of Ag-NPs which was purchased from Sigma–Aldrich (USA). Meanwhile, the sugar was used as a green reducing of silver ions to Ag atoms and was obtained from BDH Chemical Ltd., Poole, UK. All solutions were freshly prepared using double distilled water and kept in the dark to avoid any photochemical reactions. All glassware used in experimental procedures were cleaned in a fresh solution of HNO3/HCl (3:1, v/v), washed thoroughly with double distilled water, and dried before use.
Synthesis of Ag-NPs by using green method
The preparation of Ag-NPs in the PEG matrix is quite directly forward. In a typical synthesis, a 10 mL of a 1.0 M solution of AgNO3 was added to 200 mL of a 0.1 wt.% aqueous solution of soluble PEG to obtain the clear solution . After complete dissolution of these components, 20 mL of a 1.0 M aqueous solution of sugar was then added and further stirred. The solution obtained was distributed into 5 cuvettes, which were stirred and maintained at different periods of time: 1 (a), 3 (b), 6 (c), 24 (d), and 48 h (e), respectively. Throughout the reduction process, all solutions were kept at a constant temperature of 60°C in the dark to avoid any photochemical reactions. All solution components were purged with nitrogen gas prior to use. Subsequently, reduction proceeded in the presence of nitrogen to eliminate oxygen. The obtained colloidal suspensions of [Ag (PEG)] were then centrifuged at 20000 rpm for 15 min and washed four times to remove silver ion residue. The precipitate nanoparticles were then dried overnight at 40°C under vacuum overnight to obtain the Ag-NPs.
Evolution of antibacterial activity
The in vitro antibacterial activity of the samples was evaluated by utilizing the disc diffusion method using Müeller–Hinton Agar (MHA) with determination of inhibition zones in millimeter (mm), which conform with recommended standards of the National Committee for Clinical Laboratory Standards (NCCLS; now renamed as Clinical and Laboratory Standards Institute, CLSI, 2000). Salmonella typhimurium (S. typhimurium SL1344) and Staphylococcus aureus (S. aureus) (ATCC 25923) were used for the antibacterial effect assay. Briefly, the sterile paper discs (6 mm) impregnated with 20 μl of PEG, and [Ag (PEG)] (3, 6, 24 and 48 h) with different treatment times were suspended in sterile distilled water and were left to dry at 37°C for 24 h in a sterile condition. The bacterial suspension was prepared by making a saline suspension of isolated colonies selected from tryptic soy agar plate, the agar plates were grown for 18 to 24 h. The suspension was adjusted to match the tube of 0.5 McFarland turbidity standard using the spectrophotometer of 600 nm, which equals to 1.5 × 108 colony–forming units (CFU)/ml. The surface of MHA was completely inoculated using a sterile swab, which steeped in the prepared suspension of bacterium. Finally, the impregnated discs were placed on the inoculated agar and incubated at 37°C for 24 h. After incubation, the diameter of the growth inhibition zones was measured. Chloramphenicol (30 μg) and Cefotaxime (30 μg) were used as the positive standards in order to control the sensitivity of the bacteria. All tests were done in triplicate.
Characterization methods and instruments
The prepared Ag-NPs were characterized by using the X–ray diffraction (XRD), transmission electron microscopy (TEM), ultraviolet–visible spectroscopy, Fourier transform infrared (FT–IR) spectroscopy and zeta potential measurements. The XRD patterns were recorded at a scan speed of 2° min–1. Meanwhile, the structures of the produced Ag-NPs were examined using Shimadzu PXRD–6000, powder X–ray diffraction. Moreover, TEM observations were carried out using the Hitachi H–7100 electron microscopy, whereas the particle size distributions were determined using the UTHSCSA Image Tool software (Version 3.00). To make sure the formation of Ag-NPs, the colloids solutions were tested for their optical absorption property using a Shimadzu H.UV, 1650 PC UV–visible spectrophotometer over the range of 300 to 700 nm. The FT–IR spectra were however recorded over the range of 200–4000 cm−1 utilizing the Series 100 Perkin Elmer FT–IR 1650 spectrophotometer. The zeta potential measurements were also performed using a Zetasizer Nano–ZS (Malvern Instruments).
The authors thank from University Putra Malaysia (UPM) for its financial support (RUGS, Project No. 9199840). The authors are also grateful to the staff of the Department of Chemistry UPM for their help in this research, Institute of Bioscience (IBS/UPM) for technical assistance.
- Cho KH, Park JE, Osaka T, Park SG: The study of antimicrobial activity and preservative effects of nanosilver ingredient. Electrochim Acta. 2005, 51: 956-960. 10.1016/j.electacta.2005.04.071.View ArticleGoogle Scholar
- Ulkur E, Oncul O, Karagoz H, Yeniz E, Celikoz B: Comparison of silver-coated dressing (Acticoat™), chlorhexidine acetate 0.5% (Bactigrass®), and fusidic acid 2% (Fucidin®) for topical antibacterial effect in methicillin-resistant staphylococci-contaminated, full-skin thickness rat burn wounds. Burns. 2005, 31: 874-877. 10.1016/j.burns.2005.05.002.View ArticleGoogle Scholar
- Parikh DV, Fink T, Rajasekharan K, Sachinvala ND, Sawhney APS, Calamari TA, Parikh AD: Antimicrobial silver/sodium carboxymethyl cotton dressings for burn wounds. Text Res J. 2005, 75: 134-138. 10.1177/004051750507500208.View ArticleGoogle Scholar
- Rupp ME, Fitzgerald T, Marion N, Helget V, Puumala S, Anderson JR, Fey PD: Effect of silver-coated urinary catheters: Efficacy, cost-effectiveness, and antimicrobial resistance. Am J Infect Control. 2004, 32: 445-450. 10.1016/j.ajic.2004.05.002.View ArticleGoogle Scholar
- Samuel U, Guggenbichler JP: Prevention of catheter-related infections: The potential of a new nano-silver impregnated catheter. Int J Antimicrob Agents. 2004, 23: 75-78.View ArticleGoogle Scholar
- Yuranova T, Rincon AG, Bozzi A, Parra S, Pulgarin C, Albers P, Kiwi J: Antibacterial textiles prepared by RF-plasma and vacuum-UV mediated deposition of silver. Photochem Photobiol A. 2003, 161: 27-34. 10.1016/S1010-6030(03)00204-1.View ArticleGoogle Scholar
- Jeong SH, Yeo SY, Yi SC: The effect of filler particle size on the antibacterial properties of compounded polymer/silver fibers. J Mater Sci. 2005, 40: 5407-5411. 10.1007/s10853-005-4339-8.View ArticleGoogle Scholar
- Chou WL, Yu DG, Yang MC: The preparation and characterization of silver-loading cellulose acetate hollow fiber membrane for water treatment. Polym Adv Technol. 2005, 16: 600-607. 10.1002/pat.630.View ArticleGoogle Scholar
- Sun RW, Chen R, Chung NP, Ho CM, Lin CL, Che CM: Silver nanoparticles fabricated in Hepes buffer exhibit cytoprotective activities toward HIV-1 infected cells. Chem Commun. 2005, 40: 5059-5061.View ArticleGoogle Scholar
- Zhang M, Li XH, Gong YD, Zhao NM, Zhang XF: Properties and biocompatibility of chitosan films modified by blending with PEG. Biomaterials. 2002, 23: 2641-2648. 10.1016/S0142-9612(01)00403-3.View ArticleGoogle Scholar
- Luo CC, Zhang YH, Zeng XW, Zeng YW, Wang YG: The role of poly(ethylene glycol) in the formation of silver nanoparticles. J Colloid Interf Sci. 2005, 288: 444-448. 10.1016/j.jcis.2005.03.005.View ArticleGoogle Scholar
- Dobryszycki J, Biallozor S: On some organic inhibitors of zinc corrosion in alkaline media. Corros Sci. 2001, 43: 1309-1319. 10.1016/S0010-938X(00)00155-4.View ArticleGoogle Scholar
- Luo CC, Zhang YH, Wang YG: Palladium nanoparticles in poly(ethyleneglycol): the efficient and recyclable catalyst for Heck reaction. J Mol Catal A-Chem. 2005, 229: 7-12. 10.1016/j.molcata.2004.10.039.View ArticleGoogle Scholar
- Baker CN, Stocker SA, Culver DH, Thornsberry C: Comparison of the E test to agar dilution, broth microdilution and agar diffusion susceptibility testing techniques by using a special challenge set of bacteria. J Clin Microbiol. 1991, 29: 533-538.Google Scholar
- Erfani Y, Rasti A, Mirsalehian A, Mirafshar SM, Ownegh V: E-test versus disk diffusion method in determining multidrug resistant strains of Escherichia coli in urinary tract infection. Afr J Microbiol Res. 2011, 5: 608-611.Google Scholar
- Gaudreau C, Gilbert H: Comparison of disc diffusion and agar dilution methods for antibiotic susceptibility testing of Campylobacter jejuni subsp. jejuni and Campylobacter coli. J Antimicrob Chemoth. 1997, 39: 707-712. 10.1093/jac/39.6.707.View ArticleGoogle Scholar
- Manoharan A, Pai R, Shankar V, Thomas K, Lalitha MK: Comparison of disc diffusion & E test methods with agar dilution for antimicrobial susceptibility testing of Haemophilus influenza. Indian J Med Res. 2003, 117: 81-87.Google Scholar
- Clinical and Laboratory Standards Institute (CLSI): Protocols for Evaluating Dehydrated Mueller-Hinton Agar; Approved Standard-Second Edition. CSLI document M6-A2. 2006Google Scholar
- Shameli K, Ahmad MB, Zargar M, Yunus WMZW, Ibrahim NA, Shabanzadeh P, Moghaddam MG: Synthesis and characterization of silver/montmorillonite/chitosan bionanocomposites by chemical reduction method and their antibacterial activity. Int J Nanomed. 2011, 6: 271-284. 10.2217/nnm.10.161.View ArticleGoogle Scholar
- Shameli K, Ahmad MB, Yunus WMZW, Ibrahim NA, Darroudi M: Synthesis and characterization of silver/talc nanocomposites using the wet chemical reduction method. Int J Nanomed. 2010, 5: 743-751.View ArticleGoogle Scholar
- Navaladian S, Viswanathan B, Viswanath RP, Varadarajan TK: Thermal decomposition as route for silver nanoparticles. Nanoscale Res Lett. 2007, 2: 44-48. 10.1007/s11671-006-9028-2.View ArticleGoogle Scholar
- Rodriguez-Sanchez L, Blanco MC, Lopez-Quintela MA: Electrochemical synthesis of silver nanoparticles. J Phys Chem B. 2000, 104: 9683-9688. 10.1021/jp001761r.View ArticleGoogle Scholar
- Perelshtein I, Applerot G, Perkas N, Guibert G, Mikhailov S, Gedanken A: Sonochemical coating of silver nanoparticles on textile fabrics (nylon, polyester and cotton) and their antibacterial activity. Nanotechnology. 2008, 19: 245705-10.1088/0957-4484/19/24/245705.View ArticleGoogle Scholar
- Mallick K, Witcomb MJ, Scurrell MS: Polymer stabilized silver nanoparticles: A photochemical synthesis route. J Mater Sci. 2004, 39: 4459-4463.View ArticleGoogle Scholar
- Yin H, Yamamoto T, Wada Y, Yanagida S: Large-scale and size-controlled synthesis of silver nanoparticles under microwave irradiation. Mater Chem Phys. 2004, 83: 66-70. 10.1016/j.matchemphys.2003.09.006.View ArticleGoogle Scholar
- Shameli K, Ahmad M, Yunus WMZW, Rustaiyan A, Ibrahim NA, Zargar M, Abdollahi Y: Green synthesis of silver/montmorillonite/chitosan bionanocomposites using the UV irradiation method and evaluation of antibacterial activity. Int J Nanomed. 2010, 5: 875-887.View ArticleGoogle Scholar
- Shameli K, Ahmad MB, Yunus WMZW, Ibrahim NA, Gharayebi Y, Sedaghat S: Synthesis of silver/montmorillonite nanocomposite using γ-irradiation. Int J Nanomed. 2010, 5: 1067-1077.Google Scholar
- Darroudi M, Ahmad MB, Abdullah AH, Ibrahim NA: Green synthesis and characterization of gelatin-based and sugar-reduced silver nanoparticles. Int J Nanomed. 2011, 6: 569-574.View ArticleGoogle Scholar
- Raveendran P, Fu J, Wallen SL: Completely “Green” Synthesis and Stabilization of Metal Nanoparticles. J Am Chem Soc. 2003, 125: 13940-13941. 10.1021/ja029267j.View ArticleGoogle Scholar
- Vigneshwaran N, Nachane RP, Balasubramanya RH, Varadarajan PV: A novel one-pot ‘green’ synthesis of stable silver nanoparticles using soluble starch. Carbohyd Res. 2006, 341: 2012-2018. 10.1016/j.carres.2006.04.042.View ArticleGoogle Scholar
- Sharma VK, Yngard RA, Lin Y: Silver nanoparticles: Green synthesis and their antimicrobial activities. Adv Colloid Interfac. 2009, 145: 83-96. 10.1016/j.cis.2008.09.002.View ArticleGoogle Scholar
- Cao XL, Cheng C, Ma YL, Zhao CS: Preparation of silver nanoparticles with antimicrobial activities and the researches of their biocompatibilities. J Mater Sci Mater M. 2010, 21: 2861-2868. 10.1007/s10856-010-4133-2.View ArticleGoogle Scholar
- Singh A, Jain D, Upadhyay MK, Khandelwal N, Verma HN: Green synthesis of silver nanoparticles using Argemone Mexicana leaf extract and evaluation of their antimicrobial activities. Dig J Nanomater Bios. 2010, 5: 483-489.Google Scholar
- Ahmad MB, Shameli K, Yunus WMZW, Ibrahim NA: Synthesis and characterization of silver/clay/starch bionanocomposites by green method. Aust J Basic Appl Sci. 2010, 4 (7): 2158-2165.Google Scholar
- Kelly KL, Coronado E, Zhao LL, Schatz GC: The optical properties of metal nanoparticles: The influence of size, shape and dielectric environment. J Phys Chem B. 2003, 107: 668-677.View ArticleGoogle Scholar
- Stepanov AL: Optical Properties of Metal nanoparticles synthesized in a polymer by ion implantation. A review Tech Phys. 1997, 49: 143-153.Google Scholar
- Stamplecoskie KG, Scaiano JC: Light emitting diode can control the morphology and optical properties of silver nanoparticles. J Am Chem Soc. 2010, 132: 1825-1827. 10.1021/ja910010b.View ArticleGoogle Scholar
- Darroudi M, Ahmad MB, Abdullah AH, Ibrahim NA, Shameli K: Effect of accelerator in green synthesis of silver nanoparticles. Int J Mol Sci. 2010, 11: 3898-3905. 10.3390/ijms11103898.View ArticleGoogle Scholar
- Bhainsa KC, D’Souza SF: Extracellular biosynthesis of silver nanoparticles using the fungus Aspergillus fumigates. Colloids Surface B. 2006, 47: 160-164. 10.1016/j.colsurfb.2005.11.026.View ArticleGoogle Scholar
- Peng S, McMahon JM, Schatz GC, Gray SK, Sun Y: Reversing the size-dependence of surface Plasmon resonances. PNAS. 2010, 107: 14530-14534. 10.1073/pnas.1007524107.View ArticleGoogle Scholar
- Vidhu VK, Aromal A, Philip D: Green synthesis of silver nanoparticles using Macrotyloma uniflorum Spectrochimica. Acta Part A. 2011, 83: 392-397. 10.1016/j.saa.2011.08.051.View ArticleGoogle Scholar
- Zargar M, Hamid AA, Bakar FB, Shamsudin MN, Shameli K, Jahanshiri F, Farahani F: Green synthesis and antibacterial effect of silver nanoparticles using Vitex Negundo L. Molecules. 2011, 16: 6667-6676. 10.3390/molecules16086667.View ArticleGoogle Scholar
- Jacobs C, Müller RH: Production and characterization of a budesonide nanosuspension for pulmonary administration. Pharmaceut Res. 2002, 19: 189-194. 10.1023/A:1014276917363.View ArticleGoogle Scholar
- Tunc S, Duman O: The effect of different molecular weight of poly(ethylene glycol) on the electrokinetic and rheological properties of Na-bentonite suspensions. Colloid Surface A. 2008, 37: 93-99.View ArticleGoogle Scholar
- Philip D: honey mediated green synthesis of silver nanoparticles. Spectrochim Acta A. 2010, 75: 1078-1081. 10.1016/j.saa.2009.12.058.View ArticleGoogle Scholar
- Antonya JJ, Sivalingamb S, Sivaa D: Comparative evaluation of antibacterial activity of silver nanoparticles synthesized using Rhizophora apiculata and glucose. Colloids Surface B. 2011, 88: 134-140. 10.1016/j.colsurfb.2011.06.022.View ArticleGoogle Scholar
- Philip D: honey mediated green synthesis of gold nanoparticles. Spectrochim Acta A. 2009, 73: 650-653. 10.1016/j.saa.2009.03.007.View ArticleGoogle Scholar
- Ahmad MB, Tay MY, Shameli K, Hussein MZ, Lim JJ: Green synthesis and characterization of silver/chitosan/polyethylene glycol nanocomposites without any reducing agent. Int J Mol Sci. 2011, 12: 4872-4884. 10.3390/ijms12084872.View ArticleGoogle Scholar
- Chudasama B, Vala AV, Andhariya N, et al: Enhanced antibacterial activity of bifunctional Fe3O4 core-shell nanostructures. Nano Res. 2009, 2: 955-965. 10.1007/s12274-009-9098-4.View ArticleGoogle Scholar
- Chen SF, Li JP, Qian K, Xu WP: Large scale photochemical synthesis of M@TiO2 nanocomposites (M = Ag, Pd, Au, Pt) and their optical properties, CO oxidation performance, and antibacterial effect. Nano Res. 2010, 3: 244-255. 10.1007/s12274-010-1027-z.View ArticleGoogle Scholar
- Morones JR, Elechiguerra JL, Camacho A: The bactericidal effect of silver nanoparticles. Nanotechnology. 2005, 16: 2346-2353. 10.1088/0957-4484/16/10/059.View ArticleGoogle Scholar
- Lee D, Cohen RE, Rubner MF: Antibacterial properties of Ag nanoparticle loaded multilayers and formation of magnetically directed antibacterial microparticles. Langmuir. 2005, 21: 9651-9659. 10.1021/la0513306.View ArticleGoogle Scholar
- Jeong SH, Hwnag YH, Yi SC: Antibacterial properties of padded PP/PE nonwovens incorporating nano-sized silver colloids. J Mater Sci. 2005, 40: 5413-5418. 10.1007/s10853-005-4340-2.View ArticleGoogle Scholar
- Shameli K, Ahmad MB, Zargar M, Yunus WMZW, Rustaiyan A, Ibrahim NA: Synthesis of silver nanoparticles in montmorillonite and their antibacterial behavior. Int J Nanomed. 2011, 6: 581-590.View ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.